Possibilities of Integrated Fabrication of Insulation Systems in Electric Drives by Injection Molding of Thermosets

Due to the increasing demand for electro mobility and specifically for electrified vehicles, the demand for electric drive technology is expanding significantly with changing requirements in terms of the process and the application. The electrical insulation system of the stator is an essential part of the fabrication process with a high impact on the application properties. Due to limitations—for example, in terms of suitable materials for the stator insulation—a new technology of integrated fabrication by injection molding of thermosets has been founded. In this study, two epoxy (EP) types with different fillers were investigated to prove their suitability in terms of the material properties in the fabrication process and the application. A general realization of the integrated fabrication of insulation systems in electrical engineering by injection molding was proved. Further, the differences regarding the suitability of the two materials are portrayed. It was demonstrated that mainly the filler material influences the fabrication process and the properties in the application, leading to differing suitability in terms of the EP 3162 EMG within the fabrication process and in terms of XW 6640-1 within the application properties of the thermal conductivity and the thermal linear expansion. It was further shown that the filler within the material system is required to increase the thermal conductivity needed for the application. The inclusion of the filler influences the reaction kinetics and the viscosity behavior. A fabrication of the material with fillers is however still possible.


Introduction
The increasing demand for electro mobility especially in terms of electrified vehicles and powertrains is expanding the development of electric drive technology significantly. Further, the requirements not only in terms of the product but also in terms of the fabrication process is changing. To reduce the manufacturing costs and achieve economic efficiency, a high degree of automation in the production with low rejection rates is required to face the increasing demand. Concerning the product, a high power density and optimum efficiency of the electric drive unit must be reached while realizing low weight and small installation space [1]. The stator insulation system determines the power of the motor with respect to the entire life cycle of the application due to thermal and electrical restrictions [2]. Therefore, the electrical insulation system reveals a crucial position within the development of electro mobility applications.
The classic stator insulation system consists of two groups of insulation-the primary insulation covering the conductors and the secondary insulation in the slot and of the full stator by impregnation. The insulation of the conductors provides the basic electrical insulation to avoid electrical flashovers between wires, which would lead to a reduction in performance. Common insulation materials of the conductors are varnishes consisting of polyamide-imide (PAI) or foils of polyimide (PI). The foils are wrapped several times system with up to 85 mass% of fillers. These fillers allow a wide range of modifications of the material behavior and the properties achieved in the application. For example, the thermal conductivity of thermosets can be increased from 0.2 W m·K to over 2.5 W m·K [8]. The basic requirement for using thermoset injection molding for the insulation of stators is the complete impregnation of the electrical conductors by the thermoset. Impregnation is defined as the flow of a liquid through a porous medium [9]. The porous medium in the stator is covered by the windings and the slots between the conductors. With reference to [10], in the two-dimensional perspective the flow path of the liquid and thus, the impregnability is proportional to the viscosity of the liquid, the permeability of the porous medium, the impregnation time, and the processing pressure. These impact factors can be adaptable to the injection molding process with the exception of the viscosity of the liquid, since a thermoset molding compound is not a Newtonian fluid, as assumed by [10]. The complete impregnation of conductor alike structures with highly filled thermosets in the injection molding process was shown on carbon rovings by [11]. It was demonstrated that several process parameters directly influence the impregnation quality. An increasing tool temperature, for example, reduces the viscosity leading to an improvement in the impregnation and realizing complete insulation, analogous to [12]. The general use of the injection molding process to fabricate a stator has already been realized to some extent [12,13]. However, only small dimensions of the stator with short flow paths or stator segments have been implemented so far.
The aim of this paper is to investigate the suitability of epoxy-based resins for the application of insulation of stators by injection molding. The main material requirements are summarized in Table 1. The target values of these parameters are based on the standard process conditions as well as the application requirements. For example, the low viscosity is a precondition for long flow paths as this allows not only full insulation of the wires due to a high fluidity, but further a longer time with that flow path in the presence of curing parameters. The requirement for the reaction kinetics is rather complex and is therefore here not further defined. The evaluation of the reaction kinetics is presented within Section 3. The high thermal conductivity is needed with respect to the application in stator systems, as temperature rise during the usage of the stator must be dissipated easily to reduce the thermal input in the system and increase the durability. The low thermal linear expansion is based on the stator assembly, which is based on different materials such as the copper in the wire or the metal sheets in the statorette. By reaching a low thermal linear expansion, higher eligibility between the different materials is given, which increases the lifetime again. The target values in terms of the average of the partial discharge and the partial discharge inception/extinction voltage go along with the application and indicate sufficient insulation of the wires. The paper investigated two commonly used epoxy resins and reveals their general material properties as well as the fabrication of stator segments with a long flow path, to evaluate their suitability in terms of the fabrication process and the application.

Material
The experiments were conducted using two commercial types of epoxy resin (EP)-the type EP 3162 EMG (Raschig GmbH, Ludwigshafen, Germany) and the type XW 6640-1 (Duresco GmbH, Witterswil, Swizerland), which differ in terms of the anorganic filler material, but are both based on bisphenol-A. Both materials are a premixed grey-black granulate with resin, hardener, catalyst, and some carbon black pigments. The exact composition of the mixture including the filler type and grade is a business secret of Raschig GmbH or Duresco GmbH and therefore confidential. Characterization of the pure filler systems is unfortunately not possible due to the business secret. Table 2 reveals the important properties of the used material based on our own measurements. Further characterization of the material is revealed in the datasheets of the materials [14,15]. To define the properties needed for fabrication of the materials, a wide characterization of the materials was conducted in this study.  Figure 1 depicts the IR spectrum of the ATR method of the two types of epoxy resin with the main difference in the bands highlighted. The different bands are related to possible elements according to [16]. As it can be seen from the IR-spectrum there is a significant difference in the components and the proportion of resin and hardener in the two epoxy types with respect to the different bands. However, the IR spectrum is similar for the range of wavenumbers between 2.500 and 4.000 cm −1 . The difference in bands of the two epoxy types is also a clue with respect to the filler type chosen. Taking the NIST Standard reference database into account, the characteristic peak (position 3) of EP 3162 EMG suggests the use of boron nitride, whereas the characteristic peak (position 6) of XW 6640-1 depicts the use of aluminum oxide.
Both filler types are chosen mainly with respect to their high thermal conductivity, which is one of the demands in terms of the utilization of resins within the integrated fabrication of insulation systems in electrical engineering. Further, the filler in EP 3162 EMG has a high electric insulation property, which serves another demand in terms of the application. While the filler itself could not be characterized due to the business secret, the material behavior was compared to a pure epoxy resin type EP 3681 E (Raschig GmbH, Ludwigshafen, Germany), which is based on the same resin, hardener, and catalyst without fillers. The density of this type is 1.225 g/cm 3 .

Fabrication of the Test Specimens
The test samples were produced pressure controlled by a Krauss Maffei KM 80-380 CX DUR/03 injection molding machine (KraussMaffei Group, Munich, Germany) with a screw diameter of 30 mm. Two types of test samples were produced; in terms of the main material characterization, plates with the dimension of 60 × 60 × 2 [mm 3 ] were fabricated in a dual cavity to prepare the test samples needed for the different characterizations. Further, test samples-so-called single slot samples-were produced to evaluate the suitability of the material with respect to the application. The assembly of the tool is shown in Figure 2, where one stack of metal sheets together with two wires are inserted into the tool before the injection molding process starts. The cavity is sealed on the opposite side of the gate using silicone pads to ensure accessible terminals. Both filler types are chosen mainly with respect to their high thermal conductivity, which is one of the demands in terms of the utilization of resins within the integrated fabrication of insulation systems in electrical engineering. Further, the filler in EP 3162 EMG has a high electric insulation property, which serves another demand in terms of the application. While the filler itself could not be characterized due to the business secret, the material behavior was compared to a pure epoxy resin type EP 3681 E (Raschig GmbH, Ludwigshafen, Germany), which is based on the same resin, hardener, and catalyst without fillers. The density of this type is 1.225 g/cm 3 .

Fabrication of the Test Specimens
The test samples were produced pressure controlled by a Krauss Maffei KM 80-380 CX DUR/03 injection molding machine (KraussMaffei Group, Munich, Germany) with a screw diameter of 30 mm. Two types of test samples were produced; in terms of the main material characterization, plates with the dimension of 60 × 60 × 2 [mm 3 ] were fabricated The processing parameters were set as shown in Table 3. Due to different test sample volumes, the processing parameters for the two types of samples differ slightly in terms of the mold temperature and the holding pressure. However, the main parameters were kept constant for both samples.  15 15 in a dual cavity to prepare the test samples needed for the different characterizations. Further, test samples-so-called single slot samples-were produced to evaluate the suitability of the material with respect to the application. The assembly of the tool is shown in Figure 2, where one stack of metal sheets together with two wires are inserted into the tool before the injection molding process starts. The cavity is sealed on the opposite side of the gate using silicone pads to ensure accessible terminals. The processing parameters were set as shown in Table 3. Due to different test sample volumes, the processing parameters for the two types of samples differ slightly in terms of the mold temperature and the holding pressure. However, the main parameters were kept constant for both samples.

Characterization
To evaluate the suitability of the material in terms of the demand of the application the material was characterized with respect to the injection molding process, the fabrication in the test sample, and the resulting properties in the application. For each characterization a material recommendation is given respectively.

Characterization
To evaluate the suitability of the material in terms of the demand of the application the material was characterized with respect to the injection molding process, the fabrication in the test sample, and the resulting properties in the application. For each characterization a material recommendation is given respectively.

Specific Heat Capacity c According to ISO 11357-4
To evaluate the material impact, specifically due to the fillers, on the temperature control and the flow and curing process, the specific heat capacity c was determined at 25 • C using the C80 calorimeter (type: 3D-Calvet calorimeter; TA Instruments, New Castle, DE, USA). Although the specific heat capacity c is temperature dependent, the measured parameters are assumed to be valid in terms of evaluating the impact of the material on the curing.

Thermal Conductivity a According to DIN EN 821
To analyze the thermal conductivity a in terms of the process as well as the application properties, plate-like samples of the dimension 12.7 × 12.7 [mm 2 ] were prepared from the middle of the test samples of the plate. The measurements were carried out for the temperature sets of 23, 80, 120, and 160 • C, to consider the temperature dependence within the analysis. Three samples per temperature set were examined using a Nanofash (type: LFA 447; Netzsch-Group, Selb, Germany).

Thermal Linear Expansion ∆L According to ISO 7991
The thermal linear expansion ∆L was determined after the preparation of a sample with the dimension of 4 × 4 [mm 2 ] from the test sample of the plate, using a thermomechanical analyzer (type: TMA 450; TA instruments, New Castle, DE, USA). The analysis was set between −20 and 200 • C with a heating rate of 3 • C per minute. The thermal linear expansion ∆L has mainly an impact on the application properties. To investigate the temperature dependent reaction kinetics in terms of the process conditions of the material, a differential scanning calorimetry (DSC Q100; TA Instruments, New Castle, DE, USA) was used. Samples of about 5 mg were placed in DSC aluminum pans and heated with a constant rate of 10 • C per minute from 0 • C to 240 • C. The experiments were conducted in a nitrogen atmosphere with a flow rate of 50 mL per minute. To characterize the curing process, the specific enthalpy ∆H ges; 1 and the peak temperature T peak were determined. Further, the reaction turnover α was calculated considering Equation (1) where ∆H j is the specific enthalpy at the temperature T j and ∆H ges;1 is the total specific enthalpy in the first heating cycle [7].
2.3.5. Determination of the Viscosity Using a Rotational Viscometer According to DIN EN 6043 To characterize the viscosity, as one of the most important processing conditions in terms of thermosets, a rotational viscometer (Discovery Hybrid Rheometer 2; TA Instruments, New Castle, DE, USA) was used with DIN EN 6043. The viscosity was determined with respect to increasing temperature (dynamic behavior) and to time dependence (isothermal). The assembly was based on two plates with a shearing load rotating with a constant frequency of 1 Hz. In the case of the dynamic measurements, the temperature range was set between 90 • C and 200 • C with a constant heat rate of 5 • C per minute. The minimum of the viscosity η min and the corresponding temperature Tη min were analyzed.
The isothermal measurements started at a certain temperature, which was held constant, and the change of the viscosity depending on the time was determined. This isothermal plateau was set at a temperature of η min , which was 120 • C in the case of EP 3162 EMG and 110 • C for XW 6640-1, and was further increased in steps of 20 • C up to 180 • C ongoing from 120 • C. The route of the viscosity η relative to the time with respect to a constant temperature follows an s slope. The time t pot between the beginning of the calculation and the turning point-so-called pot life-was analyzed.

Microscopy
To analyze the position of the wire within the stack and the insulation of the wire due to the injection molding process, small strips of the single slot sample were removed using a water-cooled saw with minimal temperature input. The strips were taken from positions near and far away from the gate, to evaluate the change of the position of the wires and the polymer along the flow path. The strip samples were embedded in cold-curing epoxy resin (type: Epofix; Struers GmbH, Ottensoos, Germany) and polished.
Afterwards, the samples were characterized by a stereo microscope (type: Axio Zoom.V16; Carl Zeiss AG, Oberkochen, Germany) to create an overview image and further characterized by a reflected light microscope (type: Axio Imager.M2; Carl Zeiss AG, Oberkochen, Germany) to create images in more detail.

Average of Partial Discharge and Partial Discharge Inception/Extinction Voltage
The evaluation of the partial discharge (PD) and the partial discharge inception (PDIV) as well as the extinction voltage (PDEV) were realized using a test equipment with two parallel electrodes, which is defined by IEC 60243-1, and a measuring system within a of the partial discharge level, the partial discharge inception, and the extinction voltage were defined using the testing profile as shown in Figure 3. The testing time for the partial discharge inception voltage (PDIV) was defined with 15 s, and for the partial discharge level (PD) for 30 s. Further, the voltage incline was 100 V per second. The experiments were held at a room temperature of 20 • C with a humidity of 50%.
a Faraday cage according to IEC 60270 (type: Omicron MPD 600; Omicron elect GmbH, Klaus, Austria). The test samples were provided by the material supplier an the dimension of 150 × 150 × 4 [mm 2 ] in terms of EP 3162 EMG as well as 100 × 1 [mm 3 ] for XW 6640-1. As the thickness of the plates is the only dimension, which im the measurement, the different cross sections of the plates in terms of the two ma do not affect the testing. After clamping the test samples within the test setting, the of the partial discharge level, the partial discharge inception, and the extinction v were defined using the testing profile as shown in Figure 3. The testing time for the discharge inception voltage (PDIV) was defined with 15 s, and for the partial disc level (PD) for 30 s. Further, the voltage incline was 100 V per second. The experi were held at a room temperature of 20 °C with a humidity of 50%.

Specific Heat Capacity c According to ISO 11357-4
The specific heat capacity c reaches 0.997 J g· • C in terms of the material EP 3162 EMG and 0.899 J g· • C in terms of XW 6640-1. For the pure epoxy resin c reaches 1.616 J g· • C , which shows that the fillers implemented in the resin reduce the specific heat capacity c. As c should reach a high value with respect to the application, as shown in Table 1, EP 3162 EMG reveals slightly higher suitability in the application, although the difference between the two materials is less.

Thermal Conductivity a According to DIN EN 821
The thermal conductivity a, as shown in Figure 4, is reduced with increasing temperature T independent of the material. Further, the standard deviation is higher in terms of the temperature of 23 • C for both materials compared to the other temperature sets. The material XW 6640-1 reaches about 40% higher values in terms of the low temperature sets. The difference in the values between the two materials is reduced to 25% higher values for higher temperatures. Nevertheless, the material XW 6640-1 reaches higher values for a and reveals therefore higher suitability in terms of Table 1. It can be also seen that the fillers in both materials increase a compared to the pure epoxy resin, which reveals a significant lower value for a at a temperature of 23 • C.
terms of the temperature of 23 °C for both materials compared to the other temperature sets. The material XW 6640-1 reaches about 40% higher values in terms of the low temperature sets. The difference in the values between the two materials is reduced to 25% higher values for higher temperatures. Nevertheless, the material XW 6640-1 reaches higher values for a and reveals therefore higher suitability in terms of Table 1. It can be also seen that the fillers in both materials increase a compared to the pure epoxy resin, which reveals a significant lower value for a at a temperature of 23 °C.

Thermal Linear Expansion ΔL According to ISO 7991
The thermal linear expansion ΔL increases between −20 °C and 200 °C for both materials with different gradients. For low temperatures up to 60 °C, the linear route of ΔL reveals a higher gradient in terms of EP 3162 EMG, which starts at a lower value at −20 °C compared to XW 6640-1. Above 60 °C, the thermal linear expansion ΔL increases much faster in terms of EP 3162 EMG, which leads to inhomogeneous behavior over the whole temperature range. The route of the thermal linear expansion ΔL compared for both materials can be seen in Figure 5. With respect to the material requirements and Table 1, XW 6640-1 complies with the demand with a higher amount due to the lower ΔL and a more homogeneous route compared to EP 3162 EMG.

Thermal Linear Expansion ∆L According to ISO 7991
The thermal linear expansion ∆L increases between −20 • C and 200 • C for both materials with different gradients. For low temperatures up to 60 • C, the linear route of ∆L reveals a higher gradient in terms of EP 3162 EMG, which starts at a lower value at −20 • C compared to XW 6640-1. Above 60 • C, the thermal linear expansion ∆L increases much faster in terms of EP 3162 EMG, which leads to inhomogeneous behavior over the whole temperature range. The route of the thermal linear expansion ∆L compared for both materials can be seen in Figure 5. With respect to the material requirements and Table 1, XW 6640-1 complies with the demand with a higher amount due to the lower ∆L and a more homogeneous route compared to EP 3162 EMG. In comparison to the thermoset material, the stack metal sheets reveal a thermal linear expansion ΔL of 28 µ at 150 °C with only a small range over the temperature range.

Differential Scanning Calorimetry (DSC) According to ISO 11357
The route of the DSC measurements as well as the specific enthalpy ΔHges;1 and the peak temperature Tpeak (A) together with the reaction turnover α (B) are shown in Figure   Figure 5. Thermal linear expansion in the temperature range of -20 up to 200 • C compared for two EP types.
In comparison to the thermoset material, the stack metal sheets reveal a thermal linear expansion ∆L of 28 µm m at 150 • C with only a small range over the temperature range.

Differential Scanning Calorimetry (DSC) According to ISO 11357
The route of the DSC measurements as well as the specific enthalpy ∆H ges;1 and the peak temperature T peak (A) together with the reaction turnover α (B) are shown in Figure 6 in comparison for the two different EP types of EP 3162 EMG and XW 6640-1 as well as the pure epoxy resin. The reaction kinetics of the two materials with fillers reveal different values in terms of the specific enthalpy ∆H ges;1 with only 50% needed in terms of XW 6640-1 compared to EP 3162 EMG, but similar behavior regarding the reaction turnover α and the peak temperature T peak . The reaction turnover α illustrates an s slope as expected. The level of the specific enthalpy ∆H ges;1 and the peak temperature T peak is mainly influenced by the material in terms of the different heat capacity c. With that, XW 6640-1 requires less applied heat in the curing process. As the difference between the two materials within the reaction kinetics is only present in terms of the level of ∆H g es;1 , a similar behavior during the fabrication regarding the process parameters is likely. However, EP 3162 EMG depicts a higher standard deviation, leading to more unstable process conditions. Compared to the pure epoxy resin, the specific enthalpy ∆H g es;1 is significantly reduced by the fillers as they do not participate within the hardening process. As the thermal conductivity a is increased by the filler systems, the reaction turnover α is shifted to lower temperatures in terms of the filler systems compared to the pure epoxy resin. With that, the presence of the fillers in the two material systems reduces the specific enthalpy ∆H ges;1 needed for the reaction and changes the temperature of the curing with respect to the reaction turnover α.
Polymers 2022, 14, 5352 11 of 17 Figure 6. Route of DSC measurements with specific enthalpy ΔHges;1 and peak temperature Tpeak (A) as well as reaction turnover α (B) compared for two EP types and the pure epoxy resin.

Determination of the Viscosity Using a Rotational Viscometer According to DIN EN 6043
The route of the complex viscosity as dynamic behavior is shown in Figure 7A for the two different EP types. EP 3162 EMG reveals about half a decade lower viscosity relative to XW 6640-1 with a slightly higher temperature of the minimum of viscosity. After reaching the minimum of the viscosity, EP 3162 EMG increases over a small range of temperature and gains much higher values compared to XW 6640-1. Compared to the pure resin the minimum of the viscosity is increased in terms of the filler systems by at least three decades. Figure 7B further shows the pot life tpot for both EP types, where XW 6640-1 reaches higher values compared to EP 6640-1. With respect to the pure epoxy resin the pot life tpot is only increased for low temperatures. With increased temperature the difference between the material systems with and without filler is reduced. Overall, this Figure 6. Route of DSC measurements with specific enthalpy ∆H ges;1 and peak temperature T peak (A) as well as reaction turnover α (B) compared for two EP types and the pure epoxy resin.

Determination of the Viscosity Using a Rotational Viscometer According to DIN EN 6043
The route of the complex viscosity as dynamic behavior is shown in Figure 7A for the two different EP types. EP 3162 EMG reveals about half a decade lower viscosity relative to XW 6640-1 with a slightly higher temperature of the minimum of viscosity. After reaching the minimum of the viscosity, EP 3162 EMG increases over a small range of temperature and gains much higher values compared to XW 6640-1. Compared to the pure resin the minimum of the viscosity is increased in terms of the filler systems by at least three decades. Figure 7B further shows the pot life t pot for both EP types, where XW 6640-1 reaches higher values compared to EP 6640-1. With respect to the pure epoxy resin the pot life t pot is only increased for low temperatures. With increased temperature the difference between the material systems with and without filler is reduced. Overall, this results in a lower sensitivity of XW 6640-1 regarding the impact of time and temperature during the curing. As the difference in the values of t pot between the two materials is low, the significantly lower viscosity in terms of EP 3162 EMG is the crucial factor to evaluate the viscosity behavior of the two EP types. Therefore, EP 3162 EMG is defined as more suitable in terms of the flow conditions, as the low viscosity is more likely to realize long flow paths. The higher pot life t pot makes the material system more sensitive in terms of the impact of time and temperature. However, it can be used in terms of low fabrication times leading to cost reduction in the production process. The high increase of EP 3162 EMG after reaching the minimum of the viscosity refers to fast curing after reaching a certain temperature set-up. This can be used in terms of low fabrication times, however it has to be taken into account that this might also hinder the achievement of long flow paths. The low viscosity enhances the possibility of long flow paths, but fast curing reduces them.

Microscopy
The assembly of the single slot sample is shown in Figure 8 with the copper wire itself (A), the copper wire inserted into the stack metal sheets (B), which functions as the inserts in the injection molding process, and the sample after fabrication (C). The sample reveals full filling of the cavity and the possibility of sealing through silicon pads, as the material load on the copper wire stops at a defined position.

Microscopy
The assembly of the single slot sample is shown in Figure 8 with the copper wire itself (A), the copper wire inserted into the stack metal sheets (B), which functions as the inserts in the injection molding process, and the sample after fabrication (C). The sample reveals full filling of the cavity and the possibility of sealing through silicon pads, as the material load on the copper wire stops at a defined position.

Microscopy
The assembly of the single slot sample is shown in Figure 8 with the copper wire itself (A), the copper wire inserted into the stack metal sheets (B), which functions as the inserts in the injection molding process, and the sample after fabrication (C). The sample reveals full filling of the cavity and the possibility of sealing through silicon pads, as the material load on the copper wire stops at a defined position.  Further, Figure 9 depicts the position of the conductor in the cavity near the gate (A) and far away from the gate at the end of the flow path (B). It can be seen that the position of the wires changes along the flow path leading to a replacement of the conductor on the opposite side of the gating system. While the straight wire terminals are clamped near position B, the curved ends near the gating (A) remain unfixed. This change in the position might occur due to the forces of the injection process. It can be assumed that the optimization of the process parameter can reduce this movement. At this moment, full insulation of the conductor is yet not given at the end of the flow path. Further, Figure 9 depicts the position of the conductor in the cavity near the gate (A) and far away from the gate at the end of the flow path (B). It can be seen that the position of the wires changes along the flow path leading to a replacement of the conductor on the opposite side of the gating system. While the straight wire terminals are clamped near position B, the curved ends near the gating (A) remain unfixed. This change in the position might occur due to the forces of the injection process. It can be assumed that the optimization of the process parameter can reduce this movement. At this moment, full insulation of the conductor is yet not given at the end of the flow path. The details-shown in Figure 10-reveal, that general insulation in between the two wires is possible. However, the amount of material in the gap is reduced along the flow path. With that, a general insulation of the conductor using the injection molding process is possible, but further improvement has to be made in terms of the length of the flow path to ensure proper insulation along the flow path length. So far, the two EP types did not reveal a difference in the realization of the insulation and the behavior along the flow path. The details-shown in Figure 10-reveal, that general insulation in between the two wires is possible. However, the amount of material in the gap is reduced along the flow path. With that, a general insulation of the conductor using the injection molding process is possible, but further improvement has to be made in terms of the length of the flow path to ensure proper insulation along the flow path length. So far, the two EP types did not reveal a difference in the realization of the insulation and the behavior along the flow path.

Average Level of Partial Discharge and Partial Discharge Inception/Extinction Voltage
The electric strength of thermosets is crucial to ensure the suitability of the electrical machines during the application. To evaluate the qualification of the two EP types, the average level of partial discharge (PD) (A), the partial discharge inception voltage (PDIV) (B), and the partial discharge extinction voltage (PDEV) (C) are shown in Figure 11. The partial discharges should reach a low value to prevent electrical breakdowns due to degradation and to ensure the durability of the insulating material over the lifetime. With that, EP 3162 EMG has a slightly lower level of PD. By defining a margin of safety according to IEC60034-18-41 high PDIV and PDEV values ensure a safe operation of the electric machines without crucial PDs. In accordance with the PD-level the EP 3162 EMG has a higher value of PDIV and PDEV compared to XW 6640-1. It can be assumed, that the difference in the partial discharge resistance goes along with the change of the components within the two EP types which can have a decisive influence in electrical treeing inside the thermoset. Those two EPs probably do not only differ in terms of the filler type but further in terms of the amount of filler.

Average Level of Partial Discharge and Partial Discharge Inception/Extinction Voltage
The electric strength of thermosets is crucial to ensure the suitability of the electrical machines during the application. To evaluate the qualification of the two EP types, the average level of partial discharge (PD) (A), the partial discharge inception voltage (PDIV) (B), and the partial discharge extinction voltage (PDEV) (C) are shown in Figure 11. The partial discharges should reach a low value to prevent electrical breakdowns due to degradation and to ensure the durability of the insulating material over the lifetime. With that, EP 3162 EMG has a slightly lower level of PD. By defining a margin of safety according to IEC60034-18-41 high PDIV and PDEV values ensure a safe operation of the electric machines without crucial PDs. In accordance with the PD-level the EP 3162 EMG has a higher value of PDIV and PDEV compared to XW 6640-1. It can be assumed, that the difference in the partial discharge resistance goes along with the change of the components within the two EP types which can have a decisive influence in electrical treeing inside the thermoset. Those two EPs probably do not only differ in terms of the filler type but further in terms of the amount of filler. Figure 11. Average of partial discharge (PD) (A) and the partial discharge inception (PDIV) (B) as well as extinction voltage (PDEV) (C) compared for two EP types.

Conclusions
Based on the investigations of this paper, the suitability of epoxy based resins for the application of insulation of stators by injection molding could be determined. The main material requirements according to Table 1 can be divided into impact factors of the fabrication process and the application itself. It was shown that a general realization of insulation of stators by injection molding of epoxy based resins is possible. However, the EP type and regarding that, mainly the filler material influences the fabrication process and the properties in the application. In terms of the investigation, EP 3162 EMG reveals higher suitability in terms of the fabrication process and-in more detail-in terms of the low viscosity and the possibility of long flow paths, so far. However, the impact of the fast-curing process has to be taken into account, which might hinder long flow paths relative to the chosen process parameters. Further, EP 3162 EMG reveals advantages in the application due to a higher partial discharge resistance. However, this EP type has a deficiency regarding the thermal conductivity and the thermal linear expansion. The high suitability of XW 6640-1 in terms of the thermal conductivity and the thermal linear expansion could further be used by adopting the process. Further investigations are to be held in terms of the process parameters and the local definition of the copper wires position in the slot. It is assumed, that a general improvement of the insulation of the wires increases the suitability of XW 6640-1 in terms of the application. Further changes in the Figure 11. Average of partial discharge (PD) (A) and the partial discharge inception (PDIV) (B) as well as extinction voltage (PDEV) (C) compared for two EP types.

Conclusions
Based on the investigations of this paper, the suitability of epoxy based resins for the application of insulation of stators by injection molding could be determined. The main material requirements according to Table 1 can be divided into impact factors of the fabrication process and the application itself. It was shown that a general realization of insulation of stators by injection molding of epoxy based resins is possible. However, the EP type and regarding that, mainly the filler material influences the fabrication process and the properties in the application. In terms of the investigation, EP 3162 EMG reveals higher suitability in terms of the fabrication process and-in more detail-in terms of the low viscosity and the possibility of long flow paths, so far. However, the impact of the fast-curing process has to be taken into account, which might hinder long flow paths relative to the chosen process parameters. Further, EP 3162 EMG reveals advantages in the application due to a higher partial discharge resistance. However, this EP type has a deficiency regarding the thermal conductivity and the thermal linear expansion. The high suitability of XW 6640-1 in terms of the thermal conductivity and the thermal linear expansion could further be used by adopting the process. Further investigations are to be held in terms of the process parameters and the local definition of the copper wires position in the slot. It is assumed, that a general improvement of the insulation of the wires increases the suitability of XW 6640-1 in terms of the application. Further changes in the properties can be realized by different filler systems, which can-for example-even increase the thermal conductivity or the heat capacity in terms of EP 3162 EMG. The comparison of the two EP types regarding the material properties in terms of the fabrication process and the application are shown in Table 4 and reveal an intermediate result. It was also shown that the inclusion of fillers within the epoxy resin is needed to improve the thermal conductivity a. This inclusion of fillers within the material systems has an impact on the reaction kinetics and the viscosity behavior as shown. Table 4. Evaluation of the suitability of two EP types in terms of the main material requirements regarding the fabrication process and the application for the usage of thermosets to impregnate stators by injection molding [x: higher suitability; -: lower suitability].

Material Property
Qualification of the Material Further investigations plan to determine the influence of the process parameters mainly in terms of insulation of the conductor and the reduction of the change of the wire position along the flow path. Moreover, a method of defined positioning of the conductor in the slot during the fabrication process needs to be found, to use the advantages of XW 6640-1 in the application. In addition, the influence of the filler system on the process conditions and the application properties will be analyzed by integrating a defined amount of fillers in pure EP material systems.